Unidirectional fibre reinforced
geopolymer matrix composites
by Michael Welter
A thesis submitted to the Victoria University of Wellington in fulfilment of the requirements for the degree of
Doctor of Philosophy in Chemistry
Victoria University of Wellington 2013
Geopolymers have been suggested in the literature as matrix materials for fibre reinforced composites due to a unique combination of low-temperature synthesis and high temperature stability. This study investigated several key aspects of fibre reinforced geopolymer matrix composites in order to improve the basic knowledge of these materials. It was demonstrated that geopolymer matrix composites show great potential as fire-resistant materials for near room temperature applications. In particular, basalt fibre composites were of great interest due to their comparatively low cost and good mechanical performance. Microstructural investigations indicated that basalt fibres can potentially be used in geopolymer matrices up to 600°C. However, the success of the application of geopolymer matrix composites at higher temperatures is seen as critical and depends on further development of suitable matrices.
Several compositions within a sodium-metahalloysite model matrix system were evaluated in order to identify a suitable formulation for composite fabrication. An average compressive strength of ~ 79 MPa and flexural strength and modulus of ~ 10 MPa and 8.5 GPa, respectively, were achieved for the best batch of the main matrix composition. By optimising the matrix composition, the mechanical properties could be significantly improved, achieving an extremely high maximum compressive strength value of 145 MPa. Issues with reproducibility and the influence of various aspects of the fabrication process are discussed.
The room temperature flexural properties of unidirectional fibre reinforced composite bars with basalt, carbon and alumina fibres were investigated. Besides the fibre type, the effects of several other parameters including fibre sizing, matrix strength, span-to-depth ratio and specimen dimensions on the flexural properties and the failure behaviour of the composites were studied. Significant improvements to the mechanical properties were achieved with all fibre types. However, the mechanical behaviour was highly influenced by the elastic modulus of the fibre. Furthermore, it was shown that the composite properties were affected by the overall sample dimensions, the testing span and the mixing time of the geopolymer binder. The alumina fibre composites achieved the highest flexural stress with a maximum value of 470 MPa and a fibre content of ~ 30 vol.-%. Basalt and carbon fibre composites showed maximum flexural strength values around 200 MPa. Although all composite types displayed considerable post-fracture strength, only the basalt composites failed in tensile mode. The applicability of the weak matrix composites (WMC) concept to describe the mechanical behaviour of geopolymer matrix composites was discussed.
The fibre-matrix interactions were analysed between room temperature and 1000°C by means of electron microscopy, EDS and x-ray diffraction. All fibres were found to be chemically stable under the highly alkaline conditions of the geopolymer synthesis and showed no significant reaction with the geopolymer matrix at room temperature. The results indicate that basalt fibre composites may be used up to 600°C without significant degradation of the fibre. The heating of the carbon fibre composites to 600°C had drastic effect on the strength and integrity of the composite, in particular, when using sized carbon fibres. The alumina fibres showed good wetting and bonding behaviour but otherwise little reaction with the matrix even after heating to 1000°C.
I would like to thank my supervisor Prof. Ken MacKenzie for offering me the opportunity to undertake my PhD study in New Zealand, for continuously encouraging me in my own work and for the trust he put in me during these years.
I am also very thankful to Dr. Martin Schmuecker for accepting the role as co-supervisor as well as providing some of the fibre materials for this study. Despite being half way around the world, his input and support has been invaluable.
I would also like to thank the MacDiarmid Institute for providing the funding for this project. Additional funding provided through the Curtis-Gordon Scholarship, the Faculty Research Grant and the Victoria University Submission Scholarship was also greatly appreciated.
A big thank you goes to my past and present group members, in particular Brian O’Leary for all the lively discussions we had. I would also like to thank all my fellow lab members for their support and friendship over the years. In particular, I would like to thank Matthias Herzog, Martin Klimsa and Christin Gaedtke who have become great friends.
I am also very grateful to David Flynn for all the support with the electron microscopy and to Manu, Nick and Allen from the workshop who fabricated the
mixer and the moulds that were used in this study. I would also like to acknowledge Ian Minchington for letting me use the mechanical testing equipment at IRL.
I cannot thank my family enough for all their support and encouragement over the past years. I am equally indebted to Cushla, John and the rest of Roses family who have welcomed me into their family a long time ago and have since always been there for me.
My final and biggest thank you goes to my partner Rose who has always been there for me during many good and but also hard times. Without her endless love, support and encouragement, the completion of this thesis would not have been possible.
Table of contents
Abstract ... iii
Acknowledgements ... v
Table of contents ... vii
List of Figures ... xi
List of Tables ... xvii
1 Introduction ... 1
2 Background and literature review ... 7
2.1 Introduction to composite materials ... 7
2.1.1 Materials ... 9
2.1.2 Conventional fabrication methods ... 12
2.1.3 Mechanical failure behaviour of ceramic matrix composites .. 14
2.2 Geopolymers ... 18
2.2.1 Introduction ... 18
2.2.2 Terminologies ... 19
2.2.3 Materials and synthesis ... 22
2.2.4 Geopolymerisation process ... 25
2.2.5 Chemical and structural aspect of metakaolin geopolymers ... 25
2.2.6 Properties ... 28
2.3 Geopolymer matrix composites ... 31
2.3.1 Properties ... 33
3 Materials and experimental methods ... 45
3.1 Starting materials ... 45
3.1.1 Geopolymer matrix system ... 45
3.1.2 Fibres ... 47
3.2 Composition and processing of geopolymer binders ... 48
3.3 Fabrication of unreinforced specimens ... 50
3.4 Fabrication of fibre reinforced specimens ... 52
3.4.1 Preparation of fibre tapes ... 52
3.4.2 Desizing of fibres ... 53
3.4.3 Fabrication of unidirectional composite bars ... 54
3.4.4 Nomenclature for composite samples ... 56
3.5 Heat treatment ... 56
3.6 Ion exchange experiments ... 57
3.7 Characterisation methods ... 58
3.7.1 Mechanical properties ... 58
3.7.2 Electron microscopy ... 63
3.7.3 X-ray powder diffraction ... 65
3.7.4 Nuclear magnetic resonance ... 65
3.7.5 Thermal analysis – TGA/DSC ... 66
4 Characterisation of geopolymer matrices ... 67
4.1 Fabrication process and initial investigations ... 67
4.1.1 Mixing, viscosity and use-time of geopolymer binders... 67
4.1.2 Optimisation of the fabrication process ... 69
4.1.3 Drying process ... 70
4.2 Mechanical and physical properties ... 73
4.2.1 Density ... 74
4.2.2 Splitting-tensile strength ... 74
4.2.3 Compressive strength ... 76
4.2.4 Flexural strength and modulus ... 79
4.2.5 Effect of mixing time ... 81
4.2.6 Discussion ... 82
4.3 Microstructure ... 92
4.3.1 SEM and EDS ... 92
4.3.2 XRD and NMR ... 98
4.4 Thermal behaviour ... 104
4.4.1 Microstructural evolution and crystallisation ... 104
4.4.2 Thermal analysis ... 108
4.4.3 Discussion ... 109
4.5 Discussion on the reproducibility of mechanical strength with regard to fabrication process and microstructure... 110
5 Mechanical properties of unidirectional composites ... 115
5.1 Effects of fibre type and fabrication process on the flexural properties and stress-strain behaviour... 116
5.1.1 General observations and fabrication process ... 116
5.1.2 Fibre type ... 119
5.1.3 Fibre distribution in composite bars ... 125
5.2 Other factors influencing the flexural properties ... 126
5.2.1 Fibre sizing ... 126
5.2.2 Matrix composition and strength ... 128
5.2.3 Drying time ... 130
5.2.4 Specimen dimensions and span-to-depth ratio ... 131
5.3 In-plane flexural strength ... 134
5.4 Short beam shear tests ... 138
5.5 Discussion ... 139
5.5.1 The influence of fabrication process and processing variables ... 139
5.5.2 The effect of fibre type on the mechanical properties ... 142
5.5.3 Other factors influencing the mechanical properties ... 146
5.5.4 Failure behaviour of geopolymer matrix composites under flexural loading ... 149
6 Fibre-matrix interactions ... 153
6.1 Fibre Fibre-matrix interaction at room temperature ... 153
6.1.1 Chemical stability and desizing of fibres ... 153
6.1.2 Microstructural analysis of geopolymer composites ... 154
6.1.3 Discussion ... 159
6.2 Fibre-matrix interaction at elevated temperatures ... 160
6.2.1 Basalt fibre composites... 160
6.2.2 Carbon fibre composites ... 172
6.2.3 Alumina fibre composites ... 174
7 Geopolymer composites as precursors for CMCs – General
considerations and initial results ... 185
7.1.1 Ion exchange experiments ... 185
7.1.2 Discussion ... 188
8 Summary and conclusions ... 191
References ... 197
List of FiguresFigure 2.1: Boundary conditions of the relative fracture energy in relation to the elastic
mismatch of fibre and matrix for non-brittle failure behaviour after He and
Hutchinson , diagram from  ... 15 Figure 2.2: Energy dissipating mechanisms in fibre reinforced WIC-CMCs, after  ... 16 Figure 2.3: Proposed structural model for metakaolin geopolymers by Rowles et al.  ... 27 Figure 2.4: Stress-strain curves of fabric (c, d; Vf = 60 vol.-%) and unidirectional (UD)
(a, b; Vf = 70 vol.-%) fibre reinforced geopolymer composites after Foerster [3, 5]... 35 Figure 2.5: Residual strength and modulus of 3 and 6 mm thick 3k carbon fabric reinforced
geopolymer composites after heat treatment in air for one hour, after
Foden  and Lyon et al.  ... 36 Figure 2.6: Stress-strain curves of geopolymer and unidirectional carbon fibre reinforced
geopolymer composites before and after heat treatment, after He et al. .
The fibre volume content of unheated composites is 20 – 25 %. ... 39 Figure 2.7: Fracture surfaces of unidirectional carbon fibre reinforced geopolymer composites:
(a) before heat treatment, (b) heated at 1100°C, (c) heated at 1400°C, (d) interface reaction after heating at 1400°C in argon for 90 minutes, after He et al.  ... 40 Figure 3.1: Typical DTA curve (a) and particle size distribution (b) of NZCC Halloysite Premium
as specified by supplier ... 45 Figure 3.2: Morphology of dehydroxylated halloysite after calcination at 600°C over night and
screening on 353 µm sieve: a) high and b) low resolution SEM micrograph ... 46 Figure 3.3: Schematic presentation of the mixer design developed and used in this work ... 50 Figure 3.4: Moulds used for the fabrication of a) unreinforced and UD composite bars b)
Figure 3.5: Schematic fabrication process for UD fibre reinforced composite bars ... 55 Figure 3.6: Schematic of standard heating programme showing heating rates and
annealing steps ... 57 Figure 4.1: Typical weightloss of pellet specimens of compositions M1 – M4 during the drying
process under ambient conditions ... 71 Figure 4.2: Visibility of micro- and macrocracks in M1 pellets before (a) and after (b) wiping the
sample surfaces with IPA. The appearance of several microcracks in the seemingly crack free samples 1 and 4 are clearly visible ... 72 Figure 4.3: Initial evaluation of the mechanical strength of the hand mixed compositions
M1-M4 by means of splitting-tensile strength measurements ... 75 Figure 4.4: Splitting-tensile strengths of selected sample series of composition M1 subjected to
different mixing, curing and drying parameters. Several different machining and grinding preparations were tested on the four hand mixed sample batches (not further specified here). All other sample series were mechanically machined in
the same way ... 76 Figure 4.5: High magnification images of fracture surfaces, displaying typical microstructures
of well reacted areas of geopolymer compositions M1 – M5 ... 93 Figure 4.6: SEM analysis of fracture surface of M5 bar specimen: a) low magnification image
showing typical irregular surface pattern of elevated and lowered areas, largely consistent with the lighter coloured areas in backscatter image (b); c) higher magnification image showing microstructural difference between lighter area and main phase. EDS spot analyses indicate the different composition with regard to the SiO2/Al2O3 ratio of the two phases; d) EDS elemental map of image b). The blue coloured areas indicate a comparatively lower sodium and higher aluminium concentration compared to the relatively homogeneous distribution of Na, Si
and Al in the surrounding main phase ... 95 Figure 4.7: Phase inhomogeneities on fracture surface of composition M2. Arrows indicate
microstructural areas as shown in Figure 4.5-M2 ... 96 Figure 4.8: EDS mapping of various areas of fracture surface of M2 bar specimen: (a, b) low
magnification image and EDS map showing a very inhomogeneous sodium distribution. The needle structures (c) are identified as very sodium rich phases
by the EDS map (d) ... 97 Figure 4.9: X-ray diffraction patterns for geopolymer compositions M1 – M5 and metahalloysite ... 98 Figure 4.10: 27Al and 29Si MAS-NMR spectra of geopolymer compositions M1 – M5 ... 99 Figure 4.11: Microstructure and formation of small rod-like shapes in sample M1-600°C ... 105 Figure 4.12: Microstructural appearance of samples M1 (a) and M5 (b) after heating to 1000°C .... 105 Figure 4.13: Low resolution SEM image of sample M5-1000°C revealing a very
Figure 4.14: X-ray diffraction patterns for compositions M1 and M5 after heating up to 1000°C .... 107 Figure 4.15: Weighloss and DSC curves for composition M1 ... 108 Figure 5.1: Stress-strain curves recorded for the alumina, carbon and basalt composites
(top to bottom) presented in Table 5.1 ... 118 Figure 5.2: Typical stress-strain behaviour of unidirectional basalt, carbon and Nextel 610
alumina fibre reinforced geopolymer matrix composites ... 121 Figure 5.3: Typical macroscopic failure behaviour of UD composite bars made with basalt
(top), carbon (middle) and Nextel 610 alumina fibres (bottom) ... 122 Figure 5.4: Representative stress-strain curves of basalt-carbon and basalt-boron fibre
composites in comparison to basalt fibre composites ... 125 Figure 5.5: Typical fibre distribution in (a) basalt, (b, d) carbon and (c) Nextel 610 fibre
composites ... 126 Figure 5.6: Comparison of typical stress-strain behaviour of composites made from sized
and desized carbon and Nextel 610 fibres ... 128 Figure 5.7: Effect of matrix strength on the stress-strain behaviour of basalt and carbon fibre
composites ... 130 Figure 5.8: Comparison of stress-strain curves of basalt fibre composites after seven and
28 days drying time ... 131 Figure 5.9: Effect of sample thickness and span-to-depth ratio on the stress-strain
behaviour of basalt fibre composites ... 133 Figure 5.10: Typical macroscopic failure observed for UD basalt fibre composites depending
on sample thickness and span-to-depth ratio: s/d ~ 32:1, 100 mm span (top),
s/d ~ 16:1, 50 mm span (middle) and s/d ~ 16:1, 100 mm span (bottom). ... 134 Figure 5.11: Stress-strain curves recorded for in-plane and out-of-plane flexural testing
of basalt (left) and carbon (right) composites ... 136 Figure 5.12: Typical in-plane failure patterns observed for basalt (a – c) and carbon (d – f)
fibre composites ... 137 Figure 6.1: SEM micrographs of basalt fibres before (left) and after (right) exposure in
concentrated NaOH solution at 40°C for 150 h. No form of corrosive attack on the fibre surface is observed. The removal of fibre sizing is typical for all
investigated types of sized fibres ... 154 Figure 6.2: Adhesion between M1 matrix and a) basalt, b) Nextel 610, c) Nextel 610-DS and d)
carbon/carbon-DS fibres ... 155 Figure 6.3: Nextel 610-DS fibre at the transition point between a thick matrix adhesion
Figure 6.4: SEI and backscattered images of the polished surface of the M1-Basalt composite and corresponding EDS line scan profile across the fibre-matrix interface ... 157 Figure 6.5: SEI and backscattered images of the polished surface of the M1-N610 composite
and corresponding EDS line scan profile across the fibre-matrix interface ... 158 Figure 6.6: X-ray diffraction patterns of basalt fibre, M1-Basalt composite and M1
reference sample ... 158 Figure 6.7: Fracture surfaces of basalt fibre composites after heat treatment at a) 600°C,
b) 800°C and c) 1000°C ... 162 Figure 6.8: SEM micrographs of M1-Basalt composites heated to 800°C showing an embedded
fibre in the fractured composite and the matrix microstructure in an empty fibre channel. The microstructural appearance displayed in both images is equally
representative for the 600°C samples ... 163 Figure 6.9: X-ray diffraction patterns of M1-Basalt composites heated to 600 and 800°C for 1 h ... 164 Figure 6.10: SEM backscattered images of the fracture surface of the M1-Basalt composite
heated at 800°C for 1 h. EDS line scan analysis indicates the formation of an
iron-rich inner fibre reaction zone ... 165 Figure 6.11: SEM images of fracture surfaces of the M1-Basalt composite after heating to
1000°C. The images show the formation of large pores within the fibre; inhomogeneous, dense and porous matrix areas and fibre deformation within
the composite ... 166 Figure 6.12: SEM backscattered images of the polished surface of the M1-Basalt composite
after heating to 1000°C showing fibre shape accommodation and crystallisation within the fibre and EDS line scan profile across the fibre-matrix interface (see
also Figure 6.13 for EDS elemental maps) ... 167 Figure 6.13: EDS elemental maps corresponding to micrograph shown in Figure 6.12(b)
(element concentration increases from dark to bright colour) ... 168 Figure 6.14: Backscattered SEM image of fibre-matrix interface of the M1-Basalt composite
after heating to 1000°C at higher resolution with overlay of EDS line scan profile for Fe and Mg and corresponding EDS elemental maps (element concentration
increases from dark to bright colour) ... 169 Figure 6.15: Backscattered SEM image of fractured basalt fibres heated to 1000°C for 1 h ... 170 Figure 6.16: Comparison of x-ray diffraction patterns of basalt fibre, M1 matrix and M1-Basalt
composite heated to 1000°C for 1 h ... 171 Figure 6.17: Photographs of M1-C and M1-C-DS composite samples heated to 600 and 800°C ... 173 Figure 6.18: SEM micrographs of carbon fibre composite samples heated to 600°C: a) fracture
piece of sample M1-C, b) fracture surface of sample M1-C-DS, c) and d) showing different microstructural appearances of the matrix in fibre channels and fibre
Figure 6.19: Typical appearance of fibres on the fracture surface of a) M1-N610 and b) M1-N610-DS composite samples after heating to 600 and 800°C. No change in the microstructural appearance of the composite samples was observed
between the two temperatures ... 175 Figure 6.20: Examples of different microstructural appearances of fracture surfaces along
the fibre orientation representative for both M1-N610 and M1-N610-DS composites after heating to 600 and 800°C. No change in the microstructure
was observed between 600 and 800°C ... 176 Figure 6.21: SEM micrographs (a) and EDS elemental map (b) of fibres on the fractured
surface of M1-N610-DS after heating to 1000°C... 177 Figure 6.22: Backscattered SEM image with corresponding EDS elemental map and line
scan profile across the fibre-matrix interface of the polished surface of the
M1-N610 composite heated to 1000°C ... 177 Figure 7.1: Typical appearance of ion exchanged bar specimens after firing at 1000 and 1100°C ... 186 Figure 7.2: EDS maps on polished surfaces showing sodium distribution in ion exchanged
unreinforced bar (a, b) and Nextel 610 fibre reinforced composite (c, d)
specimens with M1 matrix after heating to 1000°C (Na concentration increases from black to white colour as indicated by sidebar) ... 187 Figure 7.3: Comparison of x-ray diffraction patterns of ion exchanged M1 powder samples, bar
List of Tables
Table 2.1: Formal representation of the three fundamental sialate units ... 21
Table 2.2: Reported mechanical properties and compositions of metakaolin geopolymers used as composite matrices ... 30
Table 2.3: Maximum flexural properties of selected fibre fabric reinforced geopolymer composites at room temperature ... 34
Table 2.4: Maximum flexural properties of selected unidirectional fibre reinforced geopolymer composites at room temperature ... 37
Table 2.5: Comparison of various mechanical properties of unidirectional and 3k fabric carbon fibre reinforced geopolymer composites at room temperature, after Foden  ... 38
Table 3.1: Chemical analysis of dehydroxylated halloysite ... 46
Table 3.2: Investigated fibres and relevant properties as specified by the supplier ... 47
Table 3.3: Chemical analysis of basalt fibre ... 48
Table 3.4: Component mixture and estimated molar ratios of investigated compositions ... 49
Table 3.5: Instrument settings for 29Si and 27Al MAS NMR ... 66
Table 4.1: Bulk densities of compositions M1 – M5 measured on small cylinder specimens ... 74
Table 4.2: Variability of compressive strength between different batches (including the strongest and weakest) of composition M1 all prepared by the same fabrication process and conditions ... 77
Table 4.3: Average compressive strength of the strongest batch of all matrix compositions ... 78
Table 4.5: Variability of flexural properties between different batches of composition M1 all
prepared by the same fabrication process and conditions (± standard deviation) ... 80 Table 4.6: Comparison of the flexural properties of the strongest batch of compositions
M1 – M5 ... 80 Table 4.7: Comparison between chemical composition and mechanical properties ... 84 Table 4.8: Comparison of mechanical properties of compositions M1 and M5 with other
metakaolin geopolymer matrices reported in the literature ... 88 Table 5.1: Flexural properties datasets of three exemplary composite types (M1-Basalt,
M1-Carbon, and M1-N610) to show the general influence of the order of
fabrication on the flexural strength... 117 Table 5.2: Effect of fibre type on the flexural properties of geopolymer matrix composites... 120 Table 5.3: Flexural properties of mixed basalt/carbon and basalt/boron fibre reinforced
geopolymer composites ... 124 Table 5.4: Effect of fibre sizing on the flexural properties of geopolymer matrix composites ... 127 Table 5.5: Effect of matrix strength on the flexural properties of basalt and carbon fibre
composites ... 129 Table 5.6: Effect of drying time on the flexural properties of basalt fibre composites ... 131 Table 5.7: Effect of specimen thickness and span-to-depth ratio on the flexural properties
of basalt fibre composites ... 132 Table 5.8: Comparison of in-plane and out-of-plane flexural properties of basalt and carbon
With advances in technological development, an increasing number of today’s applications call for materials with improved properties that cannot always be met by conventional bulk materials. In that regard, composite materials offer a major improvement towards the optimisation of material properties. In the most general sense, composites can be described as multiphase materials consisting of at least two distinct components. The interaction between these components results in a material with properties that cannot be obtained with any of the constituents alone. There are many different types of composites. However, for the purpose of this study, only artificial structural composites, in particular continuous fibre reinforced composites, are considered. Two main constituents of structural composites can usually be distinguished. These are generally referred to as the matrix and the reinforcement.
One of the main advantages of composite materials is the nearly unlimited combination of different materials. This opens the possibility to tailor the composite properties to meet specific application requirements. In many cases, the efforts of improving material properties are focused on improvements of the specific mechanical properties, making materials stronger, stiffer and tougher but also lighter. However, besides the mechanical performance other factors such as durability, the
required temperature stability and particularly cost play an important role in the development of new materials.
Three main classes of structural composite materials are generally distinguished according to the nature of their matrix, i.e. polymer matrix composites (PMCs), metal matrix composites (MMCs) and ceramic matrix composites (CMCs). Currently, the most common types of fibre composites are based on glass and carbon fibre reinforced polymer matrices . These composites combine high strength with light weight and relatively easy and cost-effective fabrication methods at moderately low temperatures. However, the organic nature of the matrix limits their operating temperature to about 200°C. Flammability and the development of toxic fumes and smoke may also restrict their application in some fields. For applications beyond the limitations of PMCs, metal or ceramic-based materials must be used. Ceramics generally exhibit very desirable properties such as relatively low density, high strength and stiffness, chemical stability and superior high temperature properties. However, the inherently brittle nature of ceramic materials is a major limitation for their widespread use in structural and engineering applications. This problem can be largely overcome by the incorporation of inorganic fibres to increase the toughness of the matrix and introduce a quasi-ductile, graceful failure behaviour. But despite extensive research efforts over the past decades the commercial relevance of fibre reinforced CMCs, and also MMCs, is still relatively small compared to PMCs. This can be, at least partly, attributed to the much higher overall costs of CMCs due to more complex processing requirements, higher material costs and much higher manufacturing temperatures. The high costs of CMCs may be justified in some highly demanding, high temperature applications where a specific properties profile leaves the material selection without alternative. However, for less demanding applications at temperatures below around 600 – 800°C their application becomes increasingly uneconomical. Since the application temperature of polymer based composites is limited to about 200°C, this leaves only a small number of materials, mostly metal-based, for applications in the temperature range from about 200 – 800°C. Several factors, however, such as higher density, insufficient corrosion resistance, electrical conductivity or costs may make the use of metals unfavourable
for certain applications. Therefore, new inorganic, non-metal materials that can essentially combine high strength, low density and reasonably high temperature stability in a cost-effective way for applications in this mid-temperature range would be of considerable interest.
Inorganic aluminosilicate polymers, commonly referred to as geopolymers, may offer an alternative to common ceramic and polymer matrix materials and are not subjected to some of the drawbacks of these materials. Geopolymers are synthetic inorganic compounds, generally made by reaction of aluminosilicate sources and alkali activation solutions at high pH and near ambient temperatures. The initially viscous geopolymer binders cure and harden in similar fashion to organic thermosetting resins to form a generally amorphous three-dimensional solid material with ceramic-like properties. Typically, geopolymers are characterised by low density, reasonable mechanical strength and good temperature resistance up to 1000°C. However, they are also inherently brittle. Although the mechanical properties of geopolymers are much more similar to ordinary Portland Cement (OPC) and some organic polymers rather than common engineering ceramics such as Al2O3, mullite or SiC, the unique combination of properties and low temperature processing has considerable potential in developing cost-effective inorganic composite materials. Thus, they offer an economical alternative to conventional CMCs for applications in a mid-temperature range up to ~ 800°C, effectively bridging the gap between existing PMC and CMC materials. Furthermore, geopolymer composites may also be of interest as precursors for the fabrication of true CMCs due to the typical transformation of geopolymers into crystalline ceramic phases at higher temperatures.
The idea to use geopolymers as a matrix material for fibre reinforced composites was first investigated in the 1980s with the objective to fabricate moulding tools and patterns for the plastic processing industry . Subsequently, it has been shown that the mechanical properties of geopolymers can be significantly improved by the incorporation of inorganic fibres such as carbon, silicon carbide (SiC), alumina, aluminosilicate, basalt and glass fibres [3-30]. However, despite the significant
potential of geopolymer matrix composites for structural applications suggested in the existing literature, these materials have so far received relatively little attention and have only attracted applications in some niche markets. In particular with regard to continuous fibre reinforced geopolymer composites [3-19], the published literature and property database remain scarce. One of the main reasons for this may be associated with a general scepticism against geopolymer science and technology in the past. However, geopolymer technology has established itself in recent years as a growing area of scientific interest and significant advances towards a better understanding of geopolymers have been made since the first studies on geopolymer composites. Thus, the full potential of these materials has yet to be determined.
In the present study, several key aspects of unidirectional fibre reinforced geopolymer matrix composites were investigated with the aim to improve the basic knowledge of these materials and to evaluate their general potential as cost-efficient composite materials for structural applications. One of the main problems of geopolymers is the often difficult comparability between different studies due to the use of different starting materials, matrix compositions, processing and fabrication techniques, testing methods and parameters, amongst others. Therefore, instead of focusing on one particular aspect, a broad objective was chosen for this work to allow for the direct comparison of the effects of a number of different variables on the composite properties in one comprehensive study. However, that also means that the depth to which individual parameters could be investigated was limited within the scope of this thesis.
The following four main aspects were investigated:
(i) characterisation of a model geopolymer matrix system
(ii) investigation of the effects of various parameters on the mechanical properties and failure behaviour of unidirectional fibre reinforced composites at room temperature
(iv) initial ion exchange experiments and general considerations regarding the use of geopolymer matrix composites as precursors for CMCs
Background and literature review
The following chapter provides a brief introduction to fibre reinforced composite materials. Furthermore, relevant information on geopolymers and a detailed literature review of fibre reinforced geopolymer composites are presented in order to establish the basic background for this study.
Introduction to composite materials
The technology of composite materials is one of the most important advances in materials development. In fact, many of today’s advanced technologies would be unimaginable without composite materials. However, the idea of composites is not new and many materials of natural and artificial source are effectively composites . This raises the question of what composites actually are and how they are defined. The common conception of what is considered a composite may vary considerably between different fields of research. In the most general way, a composite can be described as a material that consists of two or more dissimilar constituents. This definition, however, is quite flexible and allows the term composite to be used to describe almost anything, especially when considering at a close enough level [31, 32]. For the purpose of modern materials engineering,
composites are commonly defined as materials that: (i) consist of at least two chemically and physically distinct phases, (ii) are artificially bonded together and (iii) produce a structural material with enhanced properties that cannot be obtained with either of these phases taken separately . In practice, the involved phases can usually be distinguished into a continuous phase called the matrix and a strong disrupted phase usually referred to as the reinforcement. Several types of reinforcements can be distinguished: (i) continuous/long fibres, (ii) discontinuous/short fibres, (iii) whiskers (small elongated single crystals) and (iv) platelets and particles. Nevertheless, in the context of engineering materials the term composite is mainly used in reference to fibre reinforced materials . One of the advantages of using materials in fibrous form is their much higher strength compared to respective bulk forms. This is due to the small size of the fibres and the accompanying reduction of critical defects in the material structure. However, since the use of materials in fibre form is not applicable for most engineering purposes they need to be bonded together by a matrix to form a strong and stiff solid . Although the matrix is generally the weaker phase and dilutes the properties of the fibres to some degree, the matrix enables load transfer to the fibres and also protects them from abrasion and environmental attack . Thus, both the matrix and the fibre properties play a fundamental role in the performance of composites.
The concept of composite materials has been employed by man for thousands of years. One of the oldest examples of artificial, man-made composite materials are straw reinforced mud bricks for building purposes. A more modern example is the use of steel rods or mesh to reinforce concrete structures, a practice which finds its origins in the mid-19th century and may be seen as the origin of composite research. Nevertheless, composite materials did not become a distinct discipline of materials research until around the 1960s . The developments at that time were strongly driven by the advances in aerospace technology and composites were, for the most part, only considered for high-performance applications, thus making them quite exclusive. Today, composites are widely used and applications range from high tech aerospace constructions to body parts for cars, trains and aircrafts; high temperature, corrosion, oxidation and/or wear resistant applications for industrial processes and
sport articles . In most cases, the main reason for the use of composite materials is to improve the mechanical properties of the matrix such as strength, stiffness or toughness. Of particular interest, and a general advantage of composites, are their often high specific properties, that is, high strength and stiffness in relation to the material density. However, other properties such as the resistance to fatigue, creep, corrosion, thermal conductivity or electrical resistivity can also be modified by the incorporation of reinforcing phases [1, 35]. Ultimately, the properties of the composite are determined by the choice of reinforcement and matrix. Through the combination of different materials, the properties of the composite can be tailored to meet the specific requirements of a given application. This is a major advantage of composite materials. However, higher costs compared to conventional materials are among the disadvantages of these materials. Also, fibre composites are highly heterogeneous and generally show a marked anisotropy, i.e. the properties of the composite depend considerably on the orientation. This anisotropy has to be taken into account during the design of components.
Besides the fundamental influence of fibre and matrix, the composite properties also depend on several other key parameters including the fibre-matrix interface and its strength, the fibre content, the fibre architecture (short fibres, continuous fibres, woven fabrics), fibre orientation and the fabrication process. The fibre-matrix interface is a very critical parameter and has significant influence on the overall performance of the composite. If the interface is too weak, the load cannot be transferred onto the fibres resulting in low strength and stiffness. On the other hand, an interfacial that is too strong bond will prevent reinforcing mechanisms and cause brittle failure behaviour. The concept of fibre reinforcement of brittle matrix composites is discussed in some more detail in section 2.1.3.
A vast number of both matrix and fibre materials are currently available for the fabrication of composite materials and new or improved materials are constantly being developed. The properties and fabrication methods of the various fibres and matrix materials have been extensively studied. Comprehensive overviews on the
subject of composite materials including common fibre reinforcements and matrix materials have been published for example by Chawla , Zweben  and Cardarelli . Only some general aspects of the most commonly used fibre and matrix materials are briefly summarised here.
The fibres that are of most interest as reinforcements for composites are so-called advanced fibres. These types of fibres are generally characterised by very high strength and/or stiffness along with a low density . These fibres are typically available in form of fine diameter multifilaments or, in some cases, in form of somewhat larger monofilaments. Typical diameters of fibres used in structural composites range between approximately 5 – 150 µm. Most continuous fine diameter fibres are commercially available in a number of different forms or architectures. The most basic form for fibres is in shape of multifilament tows or rovings. A fibre tow consists of a number of more or less parallel aligned fibres. The tow size can vary significantly from several hundreds to many thousands of individual fibres. These fibres can also be used to make various styles of two- and three-dimensional woven fabrics by applying similar processes to those used in textile technology.
In general, two groups of fibres can be distinguished, i.e. organic and inorganic fibres. Inorganic fibres are of greater significance for the fabrication of high performing composites and are widely used. The most common inorganic fibre types are glass, carbon, silicon carbide, boron, alumina and aluminosilicate fibres. Inorganic fibres are typically characterised by high strength, stiffness and thermal stability. The only advanced organic fibre types that currently have any considerable relevance in polymer composites are synthetically produced aramid (e.g. Kevlar®) and to some degree high modulus polyethylene fibres [31, 34]. Organic fibres are usually cheaper than most inorganic fibres and are characterised by high strength, low density and high flexibility. However, the stiffness of organic fibres is relatively low.
As mentioned before, composite materials are often classified into three main classes according to the matrix material used. The three main groups of matrix materials are
polymers, metals and ceramic and respective composites are called polymer matrix composites (PMCs), metal matrix composites (MMCs) and ceramic matrix composites (CMCs). There are numerous types of materials in each class of matrix material that can be used for the fabrication of composites. In the following section, only polymer and ceramics materials are considered as metal-based composites are irrelevant to the present study.
Polymers are the most widely used matrix material for composites. The strength and stiffness of polymer matrices are generally relatively low. Thus, the strength and stiffness of PMCs is strongly influenced by the properties of the reinforcing fibres. Two major classes of polymers can generally be distinguished, i.e. thermosets or thermoplastics. Both types of polymers are used for the production of composites. However, thermosetting resins play a predominant role in current PMC manufacturing . Thermosets harden due to a curing reaction associated with the cross-linking of polymeric chains. The most relevant thermosetting resins for PMC manufacturing are epoxies [1, 35]. Other thermosets that are used in composites include (unsaturated) polyester and phenolics. Thermoplastics, on the other hand, soften or melt above a certain temperature but harden when cooled to room temperature. Some common examples for this type of polymers for PMCs are polyethylene, nylon, polycarbonates and polyether etherketone (PEEK) .
Ceramics are typically characterised by a number of desirable properties such as high strength, stiffness and hardness, relatively low density and good chemical resistance. However, the most important property of ceramics is their superior high temperature stability. Despite all of these highly favourable characteristics, the inherent brittleness and the accompanying catastrophic failure behaviour of ceramics limits their use in structural applications. However, this limitation can be largely overcome by incorporating fibres into the brittle ceramic matrix and carefully controlling the interaction between the two components.
Two main groups of ceramic materials are often distinguished, i.e. oxide and non-oxide ceramics. The non-non-oxide ceramics may be further specified as carbides,
nitrides or borides. Carbon is sometimes considered as a separate class of material due to its particular status and high relevance but may also be considered as a non-oxide ceramic. Alumina (Al2O3) and aluminosilicate (e.g. mullite, 3Al2O3 · 2SiO2) ceramics are by far the most important matrix materials for the fabrication of oxide ceramic composites. The choice of fibre reinforcement is usually limited to fibres of a similar chemical nature. Non-oxide CMCs are predominantly made using carbon and silicon carbide (SiC) matrices and fibres. Other inorganic, non-metallic matrix materials that are of considerable interest in composite manufacture are glasses and various cements.
2.1.2 Conventional fabrication methods
In general, the fabrication process of a composite is dictated by two factors: (i) the type and shape of the reinforcement, and (ii) the nature of the matrix . The types of fibres that are relevant to the present study are continuous fibres. Therefore, only processes involving these types of fibres are discussed here. As mentioned in the introduction of this thesis, geopolymers combine low-temperature processing similar to thermosetting resins with ceramic-like properties. Therefore, some of the general fabrication methods of thermosetting polymer-based composites are very briefly outlined below and compared to some principal aspects of ceramics manufacturing. The book “Composite Materials – Science and Engineering” by Chawla  and a list of fabrication techniques for PMCs by Cardarelli  were used as general references. For more detailed information on the manufacturing techniques of polymer and ceramic composites, the reader is referred to the specialised literature on these topics.
One of simplest and cheapest fabrication methods for PMCs is a hand lay-up. Fibres are placed into or onto a mould, and each layer is impregnated with resin using a roller. The lay-up is subsequently cured in the mould at room temperature or at slightly higher temperature in an oven. Additional pressure and/or vacuum may be applied during the curing process by using autoclaves or vacuum bagging techniques. One of the advantages of this method is the possibility to fabricate irregular shapes.
However, the quality-control is difficult and the quality of the final product depends on the skill and experience of the manufacturer.
More advanced and automated techniques include fibre winding and pulltrusion techniques. Both methods involve the passing of fibre tows through a resin impregnation bath and the subsequent removal of excess resin before forming. In case of the fibre winding process the impregnated fibres are wound onto a mandrel. Fibres can be wound parallel or in cross patterns with various angles through adjustment of different parameters. This technique is generally able to produce large cylindrical and spherical shapes. After winding, the product has to be cured in similar ways as described for hand lay-ups. The pulltrusion technique is a continuous process that allows the fabrication of relatively large shapes with a fixed cross-section such as rods or bend and flat panels. The impregnated fibre tows are pulled through a forming and curing die of the shape of the final product.
Resin transfer moulding (RTM) is an automated method that can be used to produce complex shapes. In contrast to the techniques described before, the fibres are first made into a preform which is then placed in a closed mould and is subsequently impregnated with a low viscosity resin assisted by low pressure. The product is cured by the additional application of heat.
With ceramic matrices, processing becomes generally much more complicated and expensive. The main reasons for that are all direct or indirect consequences of the high temperatures generally required for the fabrication of ceramics. There are several techniques similar to the ones described above such as filament winding or other impregnation techniques that can be used to produce green (i.e. unfired) composite parts. All of these processes are followed by some sort of sintering or hot-pressing process during which the matrix material melts or sinters, impregnates and bonds to the fibres and solidifies during cooling. The production of fibre pre-forms from continuous fibres that are subsequently infiltrated is also common for some products e.g. for SiC matrix composites. The pre-forms can be infiltrated with liquids or vapours. These techniques are called melt infiltration and chemical vapour
infiltration (CVI) respectively. However, these processes are very complex and require special equipment and technology to control the infiltration of the pre-form. In the case of dense ceramic matrices additional costly fibre coating may have to be applied.
The main advantage of polymer matrices and PMCs, respectively, over ceramic materials and the reason why PMCs find such widespread applications is the relatively low processing temperature required for the fabrication of these materials. According to Kelly and Mortensen , there are several implications that evolve from that fact: first of all, the low temperatures ease the general processing considerably and allow much simpler and cheaper tooling. Secondly, the processing does not demand much energy. All these factors have direct effect on the cost and cost-efficiency. Another advantage is that a much wider range of less expensive inorganic and organic fibres can be used. The lack of problems which often arise with high temperature processing such as chemical reactivity between fibre and matrix, complex densification methods and different thermal expansion coefficients indirectly support the relative ease of PMC processing. Thus, to increase the commercial relevance and the more widespread use of CMCs, their fabrication has to become more affordable.
2.1.3 Mechanical failure behaviour of ceramic matrix composites
The main factor limiting the use of ceramics for structural engineering applications is their inherent brittleness and low resistance to crack propagation, i.e. low fracture toughness. One possible way to improve the toughness and damage tolerance of ceramics is by the incorporation of strong and stiff fibres. However, most of the fibres used in such composites are of an inorganic nature and are also inherently brittle. In order to achieve graceful, i.e. non-catastrophic or quasi-ductile failure of the composite, the interaction between the two components has to be carefully controlled. Composite failure is usually initiated by matrix cracks above a critical stress level. To ensure damage tolerant behaviour, it is vital that the fibres remain intact as the cracks approach the fibres. This is generally achieved if the interfacial bond strength between fibre and matrix is weak enough to allow crack deflection into
the fibre-matrix interface and subsequent debonding of the fibre. The criterion for these debonding processes and the damage tolerant failure of the composite is described theoretically by He and Hutchinson  based on the critical ratio between the fracture energy of the interface ΓI and the fracture energy of the fibre ΓF in relation to the elastic mismatch between fibre and matrix, as shown in Figure 2.1.
Figure 2.1: Boundary conditions of the relative fracture energy in relation to the elastic mismatch of fibre and matrix for non-brittle failure behaviour after He and Hutchinson , diagram from 
The interfacial strength can be controlled in two different ways. Both approaches aim to prevent fibre damage based on the principle of energy dissipation of stress concentrations. The first, and more conventional, approach is the application of fibre coatings. The coatings introduce a weak interface/interphase with low crack and sliding resistance to promote crack deflection and debonding between fibre and matrix. According to Koch et al., composites based on this concept may also be referred to as weak interface composites (WIC) [37, 38]. The coatings work according to two different principles: they either bond weakly, if at all, to the surface of the fibres or they are inherently weak, e.g. by being layered or porous . Commonly applied fibre coatings for non-oxide ceramics such as SiC are carbon and boron nitride (BN). The application of fibre coatings generally becomes a necessity with increasing density and improved mechanical properties of the matrix. This is
evident from the He-Hutchinson diagram shown in Figure 2.1. The elastic modulus of the matrix increases with increasing density. For a highly dense matrix, similar elastic moduli for fibres (EF) and matrix (EM) may be assumed. Thus, a weaker interface is required in order to achieve fibre debonding and non-brittle failure behaviour and to fulfil the energy criterion ΓI / ΓF ≤ 0.25. Hence, the role of the fibre coating becomes more important. If the composite is loaded above a critical stress and the energy criterion is satisfied, then several fundamental energy dissipating mechanisms can contribute to increase the fracture toughness of the composite. The principal mechanisms that operate in WIC-CMCs during crack propagation are presented in Figure 2.2 . Due to the low fracture energy of the interface, stresses can be redistributed along the fibre-matrix interface without inducing fibre failure. As the main crack continues to propagate through the composite the fibres can bridge the crack surface behind the crack tip due to the higher strength and strain to failure of the fibres. This imposes a closure force on the crack that contributes to the increased toughness of the composite . Continued loading causes further interfacial debonding and sliding in the wake of the crack and eventually leads to fibre fracture and pull-out.
The second approach to control the fibre-matrix interaction is based on the use of porous matrices. In some ways this approach can be seen as an extension to the porous coating concept . However, in this case there is no need for fibre coatings to introduce a weak interfacial phase as the matrix itself acts as the weak phase [43, 44]. These types of composites are also called weak matrix composites (WMC) . The concept of porous matrix composites is highly attractive as it promises a simpler and more economical composite manufacturing by eliminating the need for costly fibre coatings and elaborate matrix densification methods . Porous matrix composites are of particular relevance for oxide/oxide CMCs and have been developed since the mid-1990s [39, 42, 44, 46-48]. The concept of WMCs and the reduced importance of the interfacial strength can also be displayed in Figure 2.1. Due to the dependency of the relative fracture energy ΓI / ΓF on the elastic mismatch of fibre and matrix, the ΓI / ΓF ratio can increase with increasing elastic mismatch without causing catastrophic failure. That is, with decreasing elastic modulus of the matrix, controlled through the matrix porosity, higher interfacial strength can be accepted. The porous matrix allows cracks to easily propagate through the matrix and deflect on matrix pores. This enables crack deflection close to the fibre interface and fibre debonding even in case of a strong fibre-matrix bond. The weak and porous matrix typically fails at low stresses under loading. However, local stress concentrations can be dissipated in the porous matrix through multiple matrix cracking. This allows the composites to carry significantly higher loads as long as load transfer onto the fibres is ensured. Because significant stress redistribution from the fibres to the matrix cannot take place due to the apparent weakness of the matrix, WMCs typically show large volume bundle failure of fibres as opposed to local fibre failure in WICs . The mechanical properties and behaviour of WMCs are strongly influenced by the properties and the orientation of the fibres and the loading direction. Especially under off-axis and compression loading modes, the strength of WMCs is low .
The term geopolymer was originally introduced in the 1970s by Davidovits to describe a group of newly developed amorphous to semi-crystalline aluminosilicate binder materials derived through reaction of aluminosilicate sources in aqueous alkaline media at moderately low temperatures (< 150°C) . The initial driving force behind this research was the development of new heat resistant, non-flammable and non-combustible “plastic” materials as an alternative to common organic plastics . This research eventually led to the patenting of a group of inorganic aluminosilicate binders synthesised from sodium silicate activated metakaolin . Nowadays, the term geopolymer is also applied to a range of similar aluminosilicate binders synthesised from a variety of different aluminosilicate sources such as fly ash and various alkaline activation solutions, most commonly on the basis of sodium or potassium.
The main focus of geopolymer research has been and still is on the development of geopolymers as cost-efficient construction materials, in particular as a sustainable alternative to Ordinary Portland Cement (OPC). The advantages of geopolymers compared with OPC are a much lower emission of carbon dioxide during the production process, especially when using industrial waste-materials such as fly ash as the aluminosilicate source, and potentially higher durability and strength [51, 52]. However, geopolymers have also attracted considerable interest in a wide range of other applications, e.g. in the field of structural engineering, fire resistant materials and insulations as well as for the immobilisation of toxic metals [49, 53]. Nevertheless, their widespread commercial use is limited at the current stage, mostly attracting niche markets. This is largely due to the predominantly application-oriented history of geopolymer research as indicated by the large number of patents compared to scientific publications. Also, the particular focus on traditional cement technology despite the intrinsically different nature of the chemistry of OPC and geopolymers hindered the development of a more detailed scientific understanding . A more comprehensive understanding of the reaction mechanisms and the
relationships between microstructural effects and properties of geopolymers has only been developed in recent years [54-58]. However, a complete understanding of the reaction mechanisms is essential in order to fully establish geopolymer technology and exploit the full potential of these materials.
In the previous section, geopolymers were introduced as a group of solid aluminosilicate material formed by reaction of an aluminosilicate source such as (meta-) kaolin and an alkali activation solution. However, there has been some controversy over the appropriate designation of this group of materials and as a result a variety of different names and terminologies can be found in the literature to essentially describe the same type of material [59, 60]. On the other hand, the same terms are also frequently misused for a variety of other materials involving alkali activation or mineral-based processes irrespective of the fact that their structure and properties may not correspond with the defining criteria of an actual geopolymer . This can leave the unfamiliar reader easily confused about the different terms and materials and supports scepticism towards geopolymer technology. Therefore, it is important to explicitly define the identifying characteristics of this group of materials. Some of the most common names and terminologies found in the literature are briefly discussed in the following paragraph.
The two most common designations for this group of materials found in the recent literature are the original term geopolymers and inorganic (aluminosilicate)
polymers. The latter is sometimes considered a more appropriate broad term
description . However, both terms are widely accepted among researchers today. For reasons of simplicity the term geopolymer will be adopted predominantly for this study. However, both terms may be used interchangeably throughout this work. Other terms found in the literature and referring to essentially the same materials are
alkali-bonded ceramics, chemically bonded ceramics, alkali-activated cement,
geocement, hydroceramics, low-temperature inorganic polymer glass, (poly)sialate,
and a variety of other names [3, 49, 58, 60, 62-64]. For the most part, geopolymers are defined as alkali activated aluminosilicate materials. The identifying criteria that
distinguish geopolymers from other types of alkali activated materials are the formation of a three-dimensional, largely x-ray amorphous, aluminosilicate gel framework consisting almost exclusively of tetrahedral SiO4 and AlO4- units as indicated by solid state nuclear magnetic resonance (NMR) analysis [49, 61].
The polysialate terminology was introduced in the early 1980s by Davidovits in order to describe the chemical and structural nature of geopolymers . The bonding between silicon and aluminium by bridging oxygen was described by a Si-O-Al linkage type termed sialate and a Si-O-Si linkage called a siloxo bond. The polysialate network was believed to consist of tetrahedral SiO4 and AlO4- units, linked by shared oxygen atoms, and alkali metal cations (e.g. Na+, K+). The cations, required to balance the negative charge of Al3+ in IV-fold coordination, were thought to be located in the framework cavities. A strict formalism was developed by Davidovits to envisage different structures as fundamental structural building units of the poly-condensed framework. The following empirical formula was proposed for polysialates :
Mn [-(SiO2)z-AlO2]n · w H2O
where M is an alkali cation (e.g. Na+, K+), n is the degree of polymerization and z
can attain a value of 1, 2 or 3. Hence, three main sialate building units based on the presence of only Si-O-Si and Si-O-Al linkages were distinguished in order to describe the composition of geopolymers in terms of their Si/Al ratio, see Table 2.1. These structural units or oligomers were thought to condense randomly into cross-linked chains or ring polymers to build up the x-ray amorphous framework [49, 62].
Table 2.1: Formal representation of the three fundamental sialate units
Fundamental unit Composition Si/Al Abbreviation
Sialate [− | | − − | | − −] 1 PS Sialate-siloxo [− | | − − | | − − | | − −] 2 PSS Sialate-disiloxo [− | | − − | | − − | | − − | | − −] 3 PSDS
This initial model of distinct fundamental sialate units along with Davidovits’ early work on geopolymers [49, 50, 65-67] formed the basis of the general understanding of geopolymers for many years and is therefore frequently referenced in publications prior to about the mid-2000s when introducing geopolymers. However, the practical use of this nomenclature is very limited and with an increasing scientific understanding of geopolymers seems to slowly disappearing from more recent publications. The simplicity of the polysialate model in providing a basic nomenclature and a graphic illustration of key building units forming the complex amorphous geopolymer structure is probably its main advantage. However, several aspects do not correspond to reality. For example, the strict formalism of the original model with only three structural sialate units proves inadequate to describe the possible composition range of geopolymers. Compositions with higher and non-integer Si/Al ratios are not considered despite the fact that the Si/Al ratios of many compositions in practice show non-integer values and can be well in excess of Si/Al = 3 . Nevertheless, the polysialate terminology was applied in many of the early publications on geopolymers often without providing further detail on the actual composition of the material. Thus, it is often confusing and difficult to compare the results obtained in those studies with other works. Another limitation of this nomenclature is that it provides a one-dimensional description of a three-dimensional network . Furthermore, the description of the polysialates as ring and chain polymers is not verified by experimental studies . So is the assumption that
polysialate units only comprise Si-O-Si and Si-O-Al linkages, excluding Al-O-Al linkages due to an interpretation of the Loewenstein Rule . Loewenstein’s Rule states that two tetrahedral coordinated aluminium atoms in a three-dimensional framework cannot be linked by one oxygen atom. Although the aluminium avoidance is often assumed to be strictly obeyed in tetrahedral aluminosilicate structures, it is not strictly forbidden, but rather a thermodynamic preference towards the avoidance of Al-O-Al bonds . Since Al-O-Al linkages are not strictly forbidden, they may be present to some degree in geopolymers and violate against the total exclusion in the Davidovits model. The model is also not able to predict the effect of variations of the Si/Al ratio or the type of alkali cation on the structure and the correlated properties of the material.
2.2.3 Materials and synthesis
The synthesis of geopolymers is relatively simple and generally requires two sources: (i) a reactive solid component containing sufficient amounts of reactive silica and alumina species and (ii) an alkali activation solution that contains alkali hydroxides, silicates and sometimes aluminates or combinations thereof . That generally offers a wide variety of raw materials that can be used to produce geopolymers. One of the most common geopolymer synthesis methods is the original method of Davidovits involving the reaction of a 1:1 layer-lattice aluminosilicate clay mineral such as kaolin with an alkali silicate solution under highly alkaline conditions . In most cases, the clay mineral is thermally activated prior to its use to increase its reactivity. The calcined form of kaolin is generally known as metakaolin. It has been shown that the calcination of kaolin has a significant effect on the characteristics of the geopolymer. Geopolymers formed from metakaolin show a higher reactivity and yield higher early strength, while geopolymers formed from untreated kaolin often result in weak, poorly reacted products. The degree of dehydroxylation or calcination of kaolin has been studied previously . In the metakaolin region between 550°C to about 900°C, the degree of dehydroxylation is nearly constant and the required calcination times decreases with increasing temperature. However, sinter effects can occur at higher temperatures and long annealing times, lowering the reactivity of the material. Other common aluminosilicate sources for the synthesis of geopolymers are